The amount of carbon present in plain carbon
steel has a pronounced effect on the properties of
a steel and on the selection of suitable heat
treatments to attain certain desired properties.
- Heat treatment may be defined as:
An operation or combination of operationsAn operation or combination of operations
Heating and cooling of a metal/alloy in solid stateHeating and cooling of a metal/alloy in solid state
to obtain desirableto obtain desirable
- Cause relief of internal stresses developed
during cold working, welding, casting, forging
- Harden and strengthen metals.
- Improve machinability.
- Change grain size
- Soften metals for further (cold) working as in
wire drawing or cold rolling.
- Improve ductility and toughness
- Increase , heat, wear and corrosion resistance
- Improve electrical and magnetic properties.
- Homogenise the structure to remove coring .
- Spheroidize tiny particales, such as those of
Fe₃C in steel, by diffusion.
Heat Treatment Theory
• The various types of heat-treating processes
are similar because they all involve the
heating and cooling of metals; they differ in
the heating temperatures and the cooling
rates used and the final results.
• Ferrous metals (metals with iron) are
annealing, normalizing, hardening, and
• Nonferrous metals can be annealed, but never
tempered, normalized, or case-hardened.
Stages of Heat Treatment
• Stage l—Heating the metal slowly to ensure a
• Stage 2—Soaking (holding) the metal at a
given temperature for a given period of time.
• Stage 3—Cooling the metal to room
Stages of Heat Treatment
- Internal structural changes take place.
- soaking period depends on the chemical
analysis of the metal and the mass of the part.
• Cooling Stage
- To cool the metal, you can place it in direct
contact with a COOLING MEDIUM composed
of a gas, liquid, solid, or combination of these.
• Soaking Period
Table 1: Soaking period for Hardening, Annealing and
Stages of Heat Treatment
Steel is annealed to reduce the hardness, improve
machine ability, facilitate cold-working, produce a
Full annealing is the process of softening steel by a
heating and cooling cycle, so that it may be bent or
In annealing, steel is heated above the
transformation temperature to form austenite, and
cooled very slowly, usually in the furnace.
There are several types of annealing like
black annealing, blue annealing,
box annealing, bright annealing,
flame annealing, intermediate annealing,
isothermal annealing, process annealing,
recrystallisation annealing, soft annealing,
finish annealing spheroidizing annealing
These are practiced according to their different
final product properties in the industry.
Annealing treatment can be classified into groups based on the
1.1 In full annealing the steel is heated above the critical
temperature(A3) and then cooled very slowly.
1.2 Partial annealing, also known as incomplete annealing
or intercritical annealing, involves heating of steel to a
temp. lying between lower critical temperature(A1) and
upper critical temperature (A3or Acm).
1.3 Subcritical annealing is a process in which the maximum
temp. to which is heated is always less than the lower
Classification based on phase
2.1 First-order annealing is performed on steel with the sole
aim of achieving some properties. Any change in the
characteristics of steel achieved by this type of annealing is not
correlated to phase transformation.it can be performed at a
wide range of temperatures above or below the critical
2.2 The second-order annealing differs from the former in the
sense that the end results in the former are essentially due to
phase transformation which takes place during the treatment.
Purpose of full annealing
• To relieve internal stresses
• To reduce hardness and increase ductility
• For refining of grain size
• For making the material having homogeneous
• For making the material suitable for high
• To make steel suitable for undergoing other heat
treatment processes like hardening, normalizing
3.2 Isothermal Annealing
• It is a process in which hypoeutectoid steel is heated
above the upper critical temperature and this
temperature is maintained for a time and then the
temperature is brought down below lower critical
temperature and is again maintained. Then finally it
is cooled at room temperature.
• The prefix “isothermal” associated with annealing
implies that transformation of austenite takes place
at constant temperature.
The closer the temp of isothermal holding is to A1,
coarser is the pearlite, softer is the steel, but longer is
the time of isothermal transformation.
• Improved machinability.
• Homogeneous structure and better surface finish.
• Time required for complete cycle is comparably less.
• The process is of great use for alloy steels as the steels have
to be cooled slowly.
It is suitable only for small-sized components. Heavy
components cannot be subjected to this treatment
because it is not possible to cool them rapidly and
uniformly to the holding temperature at which
transformation occurs. Thus structure wont be
homogeneous. so mechanical properties will vary
across the cross-section.
3.3 Diffusion Annealing
• This process, also known as homogenizing annealing, is employed to
remove any structural non-uniformity like dendrites, columnar grains and
chemical inhomogeneity which promote brittleness and reduce ductility
and toughness of steel.
Steel is heated sufficiently above the upper critical temperature (say,
C), and held at this temperature for 10-20 hours, followed by
Segregated zones are eliminated, and a chemically homogeneous steel is
obtained by this treatment as a result of diffusion.
Heating to such a high temp. results in considerable coarsening of
austenitic grains & heavy scale formation. The coarse austenite thus
obtained further transforms to coarse pearlite on cooling, which is not a
desirable structure as mechanical properties are impaired.
The main aim of homogenising annealing is to make the
composition uniform, i.e to remove chemical
The impact energy and ductility of the steel increase as
the homogenizing temperature increases and the
hardness, yield strength and tensile strength decrease
with an increase in the homogenizing temperature.
Homogenizing annealing has a few shortcomings as
well. It results in:
Grain coarsening of austenite, thereby impairing the properties
Thick scales on the surface of steels
It is an expensive process
3.4 Partial Annealing
• Partial annealing, also known as inter-critical
annealing or incomplete annealing, is a process in
which steel is heated between A1and Acm and is
followed by slow cooling.
• Generally, hypereutectoid steels are subjected to this
treatment. The resultant microstructure consists of
fine pearlite and cementite instead of coarse pearlite
and a network of cementite at grain boundaries.
• As low temperatures are involved in this process, it is
less expensive than full annealing.
• Hupoeutectoid steels are subjected to this treatment
to improve machinability.
• However, steels with coarse structure of ferrite and
pearlite are not suitable for this treatment. This is
because only a considerable amount of ferrite
remains untransformed, and only a part of it along
with pearlite transforms to austenite.
• This coarse or accicular untransformed ferrite
results in poor mechanical properties.
3.5 Recrystallization Annealing
• The process consists of heating steel above
the recrystallization temperature, holding at
this temperature and cooling thereafter.
• It is used to treat work-hardened parts made
out of low-Carbon steels (< 0.25% Carbon).
This allows the parts to be soft enough to
undergo further cold working without
• Recrystallization temp(Tr) is given by:
• As little scaling and decarburization occurs in
recrystallization annealing, it is preferred over full
• No phase change takes place and the final structure
consists of strain-free, equiaxed grains of fine ferrite
produced at the expense of deformed elongated
• However It would produce very coarse grains if the
steel has undergone critical amount of deformation. In
such cases, full annealing is preferred.
Aims of Recrystallization Annealing
To restore ductility
To refine coarse grains
To improve electrical and magnetic
properties in grain-oriented Si steels.
3.5 Spheroidization annealing
• Spheroidization annealing consists of heating, soaking and
cooling, invariably very slowly to produce spheroidal pearlite
or globular form of carbides in steels.
• To improve the machinability of the annealed hypereutectoid
steel spheroidize annealing is applied.
• Hypereutectoid steels consist of pearlite and cementite. The
cementite forms a brittle network around the pearlite. This
presents difficulty in machining the hypereutectoid steels.
• This process will produce a spheroidal or globular form of a
carbide in a ferritic matrix which makes the machining easy.
• Prolonged time at the elevated temperature will completely
break up the pearlitic structure and cementite network. The
structure is called spheroidite.
Spheroidizing process applied at a temperature below and above the
• Heat the part to a temperature just below the Ferrite-
Austenite line, line A1 or below the Austenite-
Cementite line, essentially below the 727 ºC (1340
ºF) line. Hold the temperature for a prolonged time
and follow by fairly slow cooling. Or
• Cycle multiple times between temperatures slightly
above and slightly below the 727 ºC (1340 ºF) line,
say for example between 700 and 750 ºC (1292 -
1382 ºF), and slow cool. Or
• For tool and alloy steels heat to 750 to 800 ºC (1382-
1472 ºF) and hold for several hours followed by slow
• All these methods result in a structure in which
all the Cementite is in the form of small globules
(spheroids) dispersed throughout the ferrite
matrix. This structure allows for improved
machining in continuous cutting operations such
as lathes and screw machines. Spheroidization
also improves resistance to abrasion.
Aims Of Spheroidization Annealing:
The normalizing of steel is carried out by
heating above the UCT (Upper Critical
Temperature) to single phase austenitic
region to get homogeneous austenite,
soaking there for some time and then cooling
it in air to room temperature.
The austenitising temperature range are:
For hypoeutectoid steels and eutectoid
• Ac3+ (40-60o
For hypereutectoid steels
• Acm + (30-50o
During normalising we use grain
refinement which is associated with
allotropic transformation upon heating
Parts that require maximum toughness
and those subjected to impact are often
When large cross sections are normalized,
they are also tempered to further reduce
stress and more closely control mechanical
The microstructure obtained by
normalizing depends on the composition
of the castings (which dictates its
hardenability) and the cooling rate.
Figure below shows the normalizing temperatures
for hypoeutectoid and hypereutectoid steels
AIMs OF NORMALIZING
• To produce a harder and stronger steel
than full annealing
• To improve machinability
• To modify and/or refine the grain structure
• To obtain a relatively good ductility
without reducing the hardness and
• Improve dimensional stability
• Produce a homogeneous microstructure
• Reduce banding
• Provide a more consistent response when
hardening or case hardening
COMPARISON OF ANNEALING AND
The metal is heated to a higher temperature and then removed
from the furnace for air cooling in normalizing rather than furnace
In normalizing, the cooling rate is slower than that of a quench-and-
temper operation but faster than that used in annealing.
As a result of this intermediate cooling rate, the parts will possess a
hardness and strength somewhat greater than if annealed.
Fully annealed parts are uniform in softness (and machinability)
throughout the entire part; since the entire part is exposed to the
controlled furnace cooling. In the case of the normalized part,
depending on the part geometry, the cooling is non-uniform resulting
in non-uniform material properties across the part.
Internal stresses are more in normalizing as compared to annealing.
Grain size obtained in normalizing is finer than in annealing.
Normalizing is a cheaper and less time-consuming process.
Comparison of temperature ranges in
annealing and normalizing
Comparison of time-temperature cycles
for normalizing and full annealing
The slower cooling of annealing results in higher temperature
transformation to ferrite and pearlite and coarser microstructures than
effect of annealing and normalizing on ductility of
Annealing and normalizing do not present a significant difference
on the ductility of low carbon steels. As the carbon content
increases, annealing maintains the % elongation around 20%. On
the other hand, the ductility of the normalized high carbon steels
drop to 1 to 2 % level.
effect of annealing and normalizing on the
tensile strength AND YIELD POINT of steels
The tensile strength and the yield point of the
normalized steels are higher than the annealed
Normalizing and annealing do not show a significant
difference on the tensile strength and yield point of
the low carbon steels.
However, normalized high carbon steels present
much higher tensile strength and yield point than
those that are annealed. This can be illustrated from
effect of annealing and normalizing on the hardness of
Low and medium carbon steels can maintain similar hardness
levels when normalized or annealed. However, when high carbon
steels are normalized they maintain higher levels of hardness than
those that are annealed.
ADVANTAGES OF NORMALIZING OVER
Better mechanical properties
Lower cost of fuel and operation
ADVANTAGES OF ANNEALING OVER
Complete absence of internal stresses which is
a necessity in complex and intricate parts
• It is the process of heating the steel to
proper austenitizing temperature , soaking at
this temperature to get a fine grained and
homogeneous austenite , and then cooling the
steel at a rate faster than its critical cooling
OBJECTIVES OF HARDENING
The aims of hardening are:
1. Main aim of hardening is to induce high hardness. The
cutting ability of a tool is proportional to its hardness.
2. Many machine parts and all tools are hardened to induce
high wear resistance higher is the hardness , higher is the
wear and the abrasion resistance .For example ,gears,
3. The main objective of hardening machine components
made of structural steel sis to develop high yield strength
with good toughness and ductility to bear high working
PROCESS OF QUENCHING
• When a heated steel object (say at 840°C) is plunged into a
stationary bath of cold it has three stages as:
Stage A -vapour-blanket stage:
• Immediately on quenching, coolant gets vapourized as the
steel part is at high temperature, and thus, a continuous
vapour- blanket envelopes the steel part.
• Heat escapes from the hot surface very slowly by radiation
and conduction through the blanket of water vapour.
• Since the vapour-film is a poor heat conductor, the cooling
rate is relatively low (stage A in fig ). This long stage is
undesirable in most quenching operations.
PROCESS OF QUENCHING
Stage B-Intermittent contact stage (Liquid-boiling stage):
• Heat is removed in the form of heat of vaporization in this
stage as is indicated by the steep slope of the cooling curve.
• During this stage, the vapour-blanket is broken intermittently
allowing the coolant to come in contact with the hot surface
at one instant, but soon being pushed away by violent boiling
action of vapour bubble.
• The rapid cooling in this stage soon brings the metal surface
below the boiling point of the coolant.
PROCESS OF QUENCHING
• The vaporization then stops. Second stage
corresponds to temperature range of 500 to◦
100 c , and this refers to nose of the CCT curve of◦
the steel , when the steel transforms very rapidly
( to non martensite product ).
• Thus, the rate of cooling in this stage is of great
importance in hardening of steels.
Stage C-Direct-Contact stage (Liquid-cooling stage):
• This stage begins when the temperature of steel
surface Is below the boiling point of coolant.
• Vapours do not form. The cooling is due to
convection and conduction through the liquid.
Cooling is slowest here.
• The oldest and still the most popular quenching medium, water meets the
requirements of low cost ,general easy availability, easy handling and
• The cooling characteristics change more than oil with the rise of
temperature, specially there is a rapid fall in cooling capacity as the
temperature rises above 60°C, because of easy formation of vapour-
• The optimum cooling pover is when water is 2O-4O°C.
• Thc cooling power of water is between brine and oils.
• Water provides high cooling power to avoid the transformation of
austenite to pearlite/bainite, but the major draw back is that it also
provides high cooling rate in the the temperature range of martensite
• At this stage, the steel is simultaneously under the influence of structural
stresses (non-uniform change in structure) and thermal stresses which
increase the risk of crack formation.
• Sodium chloride aqueous solutions of about 10% by weight are
widely used and are called brines.
• The cooling power is between 10% NaOH aqueous solution and
• These are corrosive to appliances.
• The greater cooling efficiency of brines, or other aqueous solutions
is based as :
• In brine heating of the solution at the steel surface causes the
deposition of crystal of the salt on hot steel surface .
• This layer of solid crystals disrupts with mild explosive violence,
und throws off a cloud of crystals. This action destroys the vapour-
film from the surface, and thus permits direct contact of the
coolant with the steel surface with an accompanying rapid removal
• Brines are used where cooling rates faster than water arc requited.
• Oils have cooling power between water at 40°C to water at 90°C.
• In oil-quench, considerable variation can be obtained by the use of
animal, vegetable, or mineral oil, or their blends.
• Oils should be used at 50- 80°C when these are more fluid, i.e less
VISCOUS, which increases the cooling power.
• As the oils used generally have high boiling points, moderate
increase of temperature of oil does not very much increase the
vapour blanket stage. However, oils in contrast to water, or brine,
have much lower quenching power .
• Its this relatively slow cooling rate in the range of martensitic
formation is atlvantageous as it helps in minimsing the danger to
• Oils with high viscosity are less volatile, and thus have decreased
vapour-blanket stage (increase thecooling rate). As lesser volatile
matter is lost, their cooling power is not affected much with use.
• polymer quenchants cool rapidly the heated steel to
Ms temperature, and then rather slowly when
martensite is forming .
• Polymer quenchants are water-soluble organic
chemicals of high ,molecular weights, and are
generally polyalkylene glycol-based, or polyvinyl
• Widely different cooling rates can be obtained by
varying the concentration of Organic additives in
water; higher the additions, slower is the cooling rate
• There are little dangers of distortions and cracks.
• It is an ideal quenching medium for a steel of
not very large section but with good
• Addition of O.3-O.5’% water almost doubles
the cooling capacity. Normally holding time is
2-4 minutes/cm of section thickness.
• Salt baths used for austenitising keep the steel
Tempering (formerly called drawing), consists of
reheating a quenched steel to a suitable
temperature below the transformation temperature
for an appropriate time and cooling back to room
temperature. Freshly quenched marten site is hard
but not ductile. Tempering is needed to impart
ductility to marten site usually at a small sacrifice
The effect of tempering may be illustrated as
follows. If the head of a hammer were quenched to a
fully martensitic structure, it probably would crack
after the first few blows. Tempering during
manufacture of the hammer imparts shock
resistance with only a slight decrease in hardness.
Tempering is accomplished by heating a quenched
part to some point below the transformation
temperature, and holding it at this temperature for an
hour or more, depending on its size.
The micro structural changes accompanying
tempering include loss of acicular marten site
pattern and the precipitation of tiny carbide
particles. This micro structural is referred to as
tempered marten site.